# Damaged plasticity modelling of concrete in finite element analysis

date post

09-Dec-2016Category

## Documents

view

219download

1

Embed Size (px)

### Transcript of Damaged plasticity modelling of concrete in finite element analysis

9th International Conference on Fracture Mechanics of Concrete and Concrete Structures

FraMCoS-9 V. Saouma, J. Bolander and E. Landis (Eds)

1

DAMAGED PLASTICITY MODELLING OF CONCRETE IN FINITE ELEMENT

ANALYSIS OF REINFORCED CONCRETE SLABS

AIKATERINI S. GENIKOMSOU*AND MARIA A. POLAK

*

University of Waterloo

Waterloo, ON CANADA

e-mail: agenikom@uwaterloo.ca

University of Waterloo

Waterloo, ON CANADA

e-mail: polak@uwaterloo.ca

Key words: Concrete Damaged Plasticity model, Finite Element Analysis, Punching shear,

Concrete slabs

Abstract: Two interior slab-column connections, previously tested, are analysed using 3D

nonlinear finite element methods. These slabs were tested under vertical monotonically increasing

imposed displacement through the column till failure. One slab specimen was without shear

reinforcement that failed in punching shear, while the other slab had punching shear reinforcement

and failed in flexure. Both specimens are analysed using the concrete damaged plasticity model

offered in ABAQUS. Concrete damaged plasticity model is employed with the fictitious crack

model based on the fracture energy; where different failure mechanisms are predicted for tension

and compression. Damage can be introduced in the model and it is defined separate in compression

and tension. The model can be also equipped with viscoplastic regularization that provides

additional ductility in the structure and helps to overcome convergence problems that have been

created by cracking and strain localization that relies on the smeared crack approach. Parametric

investigation based on the material and plasticity parameters is performed for the specimen without

shear reinforcement. All numerical results are compared to the test results in terms of load-

deflection responses and crack patterns. Finite element analysis results are in good agreement with

the experimental results and can give an insight into the failure mechanisms and crack

developments of each slab. The predictive capability of the calibrated models confirms their ability

for parametric studies examining the punching shear behaviour of reinforced concrete slabs with

and without shear reinforcement.

1 INTRODUCTION

Punching shear is caused by a transfer

mechanism of shear forces from the slab to the

connection and occurs within the discontinuity

D-region, where the 3D state of stresses is

complex. When the shear stresses exceed the

slabs shear capacity, punching occurs. An

inclined crack forms around the column and

the punching shear cone appears, where the

column separates from the slab.

Finite Element Analysis (FEA) of

reinforced concrete slabs can give an insight

into the slabs behaviour by predicting the

possible failure modes, supporting the

DOI 10.21012/FC9.006

mailto:agenikom@uwaterloo.camailto:polak@uwaterloo.ca

Aikaterini S. Genikomsou and Maria A. Polak

2

experimental conclusions and finally

extending these conclusions where the test

measurements are not known. Many

researchers have conducted FEA of reinforced

concrete slabs [1,2]; however, FEA of shear

reinforced slabs is limited due to the

complexity of modelling the punching shear

reinforcement.

In this paper, two reinforced concrete slabs,

one without and the other with shear

reinforcement, are analyzed using the

ABAQUS FEA software [3]. The concrete is

modelled with the concrete damaged plasticity

model.

2 TEST SPECIMENS

Two interior reinforced concrete slab-

column connections that were previously

tested by Adetifa and Polak (2005) [4] are

analyzed. Both slabs were tested under static

loading through the column stub. The

dimensions of the slabs in plan are 1800x1800

mm with simple supports at 1500x1500 mm.

The dimensions of the columns are 150x150

mm and are extended 150 mm from the top

and the bottom faces of the slabs. The

thickness of the slabs is 120 mm and the

effective depth is equal to 90 mm. The

dimensions of the slabs and the loading

process are presented in Figure 1. The flexural

reinforcement consists of 10M bars that are

placed at distance 100 mm in tension side and

200 mm in compression side. Slab SB1 has no

shear reinforcement, while SB4 is retrofitted

with four rows of shear bolts (see Figure 1).

The material properties of concrete and

reinforcement are shown in Table 1 and Table

2, respectively. Table 3 presents the test

results. Specimen SB1 failed in punching

shear at a load of 253 kN, while slab SB4

failed in flexure at a load of 360 kN. Figure 2

shows the test results for both slabs in terms of

load-deflection, while Figures 3 and 4 present

the crack pattern at failure of slab SB1 and

SB4, respectively.

Figure 1: Schematic drawing of the slabs.

Table 1: Material properties of concrete of the slabs

Slab f'c

(MPa)

f't

(MPa)

Gf*

(N/mm)

Ec

(MPa)

SB1 44 2.2 0.082 36483

SB4 41 2.1 0.077 35217 * Based on the CEB-FIP Model Code 1990

Table 2: Material properties of steel of the slabs

Slab fy

(MPa)

ft

(MPa)

Es (MPa)

fy,bolts

(MPa)

SB1 455 620 200000 -

SB4 455 620 200000 381

Table 3: Test results

Slab No. of

rows of

bolts

Failure

load

(kN)

Failure

displacement (mm)

Failure

mode

SB1 0 253 11.9 Punching

SB4 4 360 29.8 Flexure

Aikaterini S. Genikomsou and Maria A. Polak

3

Figure 2: Load versus displacement (test results).

Figure 3: Crack pattern of slab SB1.

Figure 4: Crack pattern of slab SB4.

3 FINITE ELEMENT MODELLING

The FEA simulations are performed with

the ABAQUS software. A short description of

the concrete modelling is given and all the

modelling assumptions are described below.

3.1 Concrete Damaged Plasticity model

The concrete damaged plasticity model

considers both the tensile cracking and

compressive crushing of concrete as possible

failure modes [5]. The yield function of the

concrete damaged plasticity model considers

the effective stress space, where the effective

stress is defined as: =

(1)= (

), where denotes the initial modulus of elasticity, is the equivalent plastic strain and is the damage variable that denotes the stiffness degradation.

Viscoplastic regularization according to the

Duvaut-Lions approach can be defined in the

concrete damaged plasticity model. By

introducing the viscous parameter () the plastic strain tensor is upgraded and the

damage is deduced using additional relaxation

time. The plastic potential function, that is

employed in the model, is a non-associated

Drucker-Prager hyperbolic function in which

the definition of the dilation angle is needed.

For the visualization of cracking, concrete

damaged plasticity model assumes that the

cracking starts at points where the tensile

equivalent plastic strain is bigger than zero and

the maximum principal plastic strain is

positive. The direction of the cracking is

assumed to be parallel to the direction of the

maximum principal plastic strain and it is

viewed in the Visualization module of

ABAQUS/CAE.

Concrete in tension can be characterized by

a stress-crack displacement response instead of

a stress-strain relationship due to its brittle

behaviour. The stress-crack displacement

relationship can be described with different

options: linear, bilinear or exponential tension

softening response (Figure 5).

The exponential stiffening curve can be

calculated according to Cornelissen et al.,

1986 [6] where the following equations should

be considered:

= () ( )()

() = (1 + (1

)

3

) (2

)

0

50

100

150

200

250

300

350

400

0 5 10 15 20 25 30 35 40

Lo

ad

(kN

)

Deflection (mm)

SB1

SB4

Aikaterini S. Genikomsou and Maria A. Polak

4

= 5.14

(1)

where 1 and 2 are material constants and can be considered equal to 3 and 6.93 for

normal concrete, respectively.

The fracture energy of concrete () represents the area under the tensile stress-

crack displacement curve. The fracture energy

is related to the concretes strength and

aggregate size and can be calculated using Eq.

(2) (CEB-FIP Model Code 1990) [7].

=(/)0.7 (2)

According to CEB-FIP Model Code 1990,

= 10 , is the mean value of the compressive strength associated with the

characteristic compressive strength (), ( = + 8 ) and is the base fracture energy that depends on the maximum

aggregate size, . The value of the base fracture energy can be obtained from the CEB-FIP Model Code 90 and for example for

an aggregate size () equal to 10 mm, is equal to 0.026 N/mm. In Table 1 the values

of the fracture energies for both slabs are

given. The new CEB-FIP Model Code 2010

[8] considers a different equation to calculate

th

*View more*